IS- T--18 58
by Flumerfelt, Joel F.
PHD Thesis submitted to Iowa State University
Ames Laboratory, U.S. DOE Iowa State University Ames, Iowa 50011
February 12, 1999
PREPARED FOR THE U.S. DEPARTMENT OF ENERGY
UNDER CONTRACT NO. W-7405-Eng-82.
This report was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor any agency thereof, nor any of their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise, does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.
This report has been reproduced directly from the best available copy. AVAILABILITY: To DOE and DOE contractors: Office of Scientific and Technical Information P.O. Box 62 Oak Ridge, TN 37831 prices available from: (615)576-8401 FTS: 626-8401 To the public:
National Technical InformationService U.S. Departmentof Commerce 5285 Port Royal Road Springfield, VA 22161
DISCLAIMER Portions of this document may be illegible in electronic image products. Images are produced from the best available original document.
TABLE OF CONTENTS ABSTRACT
CHAPTER 1. INTRODUCTION CHAPTER 2. BACKGROUND Aluminum Powder Production Gas atomization Processing effects Aluminum Powder Characterization Bulk chemistry Aluminum powder surface characterizations Explosibility of aluminum powders Consolidation of Aluminum Powders Press and high interparticle shear consolidation
Press and sinter consolidation
Die pressing Sintering Aluminum Alloys, Reinforcement Phases, and Mechanical Properties Extrinsic dispersoids: Composites Intrinsic dispersoids: Rapidly solidified alloys ANew "Hope" Gas Atomization Reaction Synthesis CHAPTER 3. EXPEEUMENTAL PROCEDURES Gas Atoniization Experiments Atomizer configuration Atomization parameters Metallographic Sample Preparation Powder Characterization of Powders Screened at -45 pm Diameter Powder shape and size distribution Pycnometry measurements Differential thermal analysis (DTA) Bulk powder chemistry Auger electron spectroscopy (AES) Quadrupole mass spectroscopy (QMS) X-ray diffraction (XRD) of AI-Ti-Y powder Transmission electron spectroscopy (TEM) Powder oxidation
Powder Consolidation Consolidation sequence Post consolidation heat treatment Mechanical Property Measurements Punch testing CHAPTER 4. EXPEEUMENTAL RESULTS Powder Characterization of -45 pm Diameter As-atomized Powders Shape and size distribution Density measurements and specific surface area
4 4 4 8 11 11 13 16 18 18
22 23 27 27 28
29 32 32 32 34 35 36 36 36 37 37 38 39 42 43
49 49 51 51 51
iv Pure aluminum powder analytical characterization Bulk chemistry Differential thermal analysis (DTA) Quadrupole mass spectroscopy (QMS) A E S Oxide thickness Transmission electron microscopy (TEM) Aluminum alloy powder characterization Al-Ti-Y aluminum alloy powder Al-Cu-Mg alloy powder
Powder oxidation behavior
55 57 59 69
Powder explosibility Powder Consolidation Air sintering of aluminum powders CIP-VHD-HIP and CIP-VCD-HIP consolidation Heat treatment of CAA consolidated samples Punch Test
91 95 95 95 104 106
CHAPTER 5. DISCUSSION Gas Atomization Powder Characterization Bulk oxygen measurements GARS Aluminum powder oxidation Pure aluminum powder GARS Al-Ti-Y aluminum alloy powder Aluminum powder explosibility Aluminum Powder Consolidation Tap densify and air sinter CIP-VHD-HIP and CIP-VCD-HIP consolidation Aluminum alloy powder consolidation Punch testing
113 113 124 124 129 129 133 136 138 138 139 141 142
CHAPTER 6. CONCLUSIONS
ABSTRACT In recent years, the aluminum powder industry has expanded into non-aerospace applications. However, the alumina and aluminum hydroxide in the surface oxide film on aluminum powder require high cost powder processing routes. A driving force for this research is to broaden the knowledge base about aluminum powder metallurgy to provide ideas for fabricating low cost aluminum powder components. The objective of this dissertation is to explore the hypothesis that there is a strong linkage between gas atomization processing conditions, as-atomized aluminum powder characteristics, and the consolidation methodology required to make components from aluminum powder. The hypothesis was tested with pure aluminum powders produced by commercial air atomization, commercial inert gas atomization, and gas atomization reaction synthesis
(GARS). The commercial atomization methods are bench marks of current aluminum powder technology. The GARS process is a laboratory scale inert gas atomization facility.
A benefit of using pure aluminum powders is an unambiguous interpretation of the results without considering the effects of alloy elements. A comparison of the GARS aluminum powders with the commercial aluminum
powders showed the former to exhibit superior powder characteristics. The powders were compared in terms of size and shape, bulk chemistry, surface oxide chemistry and structure, and oxide film thickness. Minimum explosive concentration measurements assessed the dependence of explosibility hazard on surface area, oxide film thickness, and gas atomization processing conditions. The GARS aluminum powders were exposed to different relative humidity levels, demonstrating the effect of atmospheric conditions on post-atomization oxidation of aluminum powder. An Al-Ti-Y GARS alloy exposed in ambient air at different temperatures revealed the effect of reactive alloy elements on post-atomization powder
vi The pure aluminum powders were consolidated by two different routes, a conventional consolidation process for fabricating aerospace components with aluminum powder and a proposed alternative. The consolidation procedures were compared by evaluating the consolidated microstructures and the corresponding mechanical properties. A low temperature solid state sintering experiment demonstrated that tap densified GARS aluminum powders can form sintering necks between contacting powder particles, unlike the total resistance to sintering of commercial air atomization aluminum powder.
CHAPTER 1. INTRODUCTION Powder metallurgy (P/M) has become important processing method for producing metals parts, because of its high efficiency in moderate to high volume production of net or near-net shapes. Additional advantages of P/M include uniform properties: fine grain structures, and chemical homogeneity. Current consumer products have an increasing number of P/M components and are found in automotive, aerospace, and non-vehicular applications. In automotive applications, ferrous-based P/M parts predominate over all other available P/M materials. However, non-ferrous P/M components are replacing ferrous components for a number of reasons, for example: weight reduction, equal or superior strength to weight ratios, and potential reduction of production costs. The United States government regulations have compelled automobile manufacturers
to improve fuel efficiencies and reduce emissions. To help meet these regulations, the automotive manufactures are exploring the use of powdered aluminum alloys and powdered aluminum metal matrix composites as substitutes for some incumbent ferrous materials in drive train components. The intrinsic properties of aluminum, for example, density and melting temperature, offer attractive incentives for weight reduction and lower metal working temperatures, which translates to lower cost. However, the automotive makers are hesitant to be solely dependent on aluminum P/M processing. For instance, in order for aluminum P/M parts to be practical for use in automobile drive train components, adequate mechanical properties, e.g., fatigue properties, are necessary. Another major issue reducing current costs of aluminum powder production and consolidation. aluminum ~ P/M processing includes aluminum powder Since the early 1 9 6 0 ’ ~
production by gas (air) atomization and powder consolidation into billets for extruding, forging, or rolling into plate or sheet [ 11. A major problem with the consolidation of the aluminum powder, particularly during pressing and sintering operations, was due to the
2 obtrusive and intrinsic oxide film on aluminum powder particle surfaces. In the early to mid-
198O's, when high-strength aluminum P/M alloys were consolidated into aerospace components, changes transpired in gas atomization practices to reduce oxide film thicknesses on aluminum powders. Inert gas atomization was deemed an alternate method to air atomization and successfully reduced surface oxide film thicknesses. Today, in addition to aerospace uses, aluminum P/M has the opportunity to penetrate broadly into high volume production of automotive components. To enhance the viability of the aluminum powder production and consolidation technologies, the process needs further
refinement to reduce manufacturing costs. An investment of time and money should lead to improvements of the current aluminum P/M technology. The expected outcome of these advances would be improvements in the quality of P/M components and reduction of manufacturing costs. To facilitate the necessary research, consortia and conferences provide a forum whereby technical information can be exchanged between the powder producers, part manufactures, and the automotive industry. Throughout my research, personal active involvement within the United States Automotive Manufacturers Partnership (USAMP) consortium and powder metallurgy conferences have facilitated the opportunity to present various aspects of the aluminum P/M research presented in this dissertation. A literature survey of aluminum P/M shows that many researchers have explored
aluminum alloy powder production practices, aluminum alloy powder characteristics, and aluminum alloy powder consolidation methods. However, there is significantly less information available about pure aluminum powders. Yet, some researchers discuss their results with the assumption that the alloy powders behave as pure aluminum powders and do not fully consider the resultant effects of the alloy elements. A benefit of studying pure aluminum P/M is that the results are unambiguous. The
outcome from this research is an extensive database upon which one can more accurately
assess the results observed in the aluminum alloy powders. Therefore, the objective of this research was to broaden the knowledge base of aluminum P M through a fundamental study of processing pure aluminum powder. To achieve this objective, four topics were
investigated: assessment of current gas atomization methods used to produce aluminum powder; powder characterizations of the resulting pure aluminum powders; consolidation of the pure aluminum powders; microstructure and mechanical property analysis of the consolidated powder samples.
CHAPTER 2. BACKGROUND Aluminum Powder Production Gas atomization
Industrial production of pure aluminum and aluminum alloy powders typically involves either commercial air atomization (CAA) or commercial inert gas atomization (CIGA). In either case, the direction of molten metal atomization is either horizontal or vertical. The selection of atomizing position depends on the desired production rate of powder and the powder size distribution. Williams  comments on three different atomization positions. The vertically upward design, Figure 2. l a and Figure 2.lb, which uses an aspirating mechanism of the aluminum melt to induce upward liquid metal flow, produces a wide particle size distribution at high production rates. The vertically downward position, Figure 2.2a and Figure 2.2b, relies on the liquid metal head pressure for downward fluid flow, has better control over the powder size distribution, but slower production rates than the vertically upward design. The horizontal system can use either the aspirating design
or metal head pressure to induce flow of the molten metal. The horizontal set-up produces medium to coarse powder size distributions. The remainder of this document will concentrate on vertical gas atomization designs, both capable of the fine powder production that is the focus of this study. The vertically upward system is used by Alcoa at the gas atomization facility in Rockdale, Texas, for CAA of aluminum powders. Before atomization, the spray chamber is purged with a gas similar to the atomization gas composition to minimize undesirable gases, such as water vapors. The molten metal is prepared in a holding furnace and transferred to the atomization melt chamber. The liquid metal has a superheat of 100°C to 150°C to eliminate the possibility of the molten aluminum freezing in the pour tube before the melt exits into the spray chamber. Gas nozzles encircle the pour tube and are focused such that
the compressed dry air  impinges upon the molten stream, disintegrating the liquid metal into droplets. Immediately after the melt break-up, cooling air from the ambient atmosphere enters the spray chamber to cool the molten droplets and passivate the surface of the droplets with an oxide film . The intent of the passivation process is to purposely oxidize the aluminum powders in an effort to minimize powder explosions during post-atomization powder handling. The cooling air may not have a low enough dew point to minimize
To Powder Collection
To Powder Collection
Co ling l w
c o ling l w
Figure 2.1. a) Schematic of vertically upward atomization system used by Alcoa for CAA of aluminum powders . b) Schematic of vertically upward atomization system used by Alcan-Toyo America for CIGA-ATA of aluminum powders [ 2 , 6 ] .
0He + O2
0 UHP N1
Exhaust apd Recirculation
5Collection X y
Figure 2.2. a) Schematic of vertically downward atomization system used by Valimet for CIGA-VAL aluminum powders . b) Schematic of vertically downward atomization system used for GARS aluminum powder processing. hydration of the oxide film . For a point of reference, Bohlen et al.  state in their paper that the air atomized process used by Alcoa to produce a 7091 aluminum alloy powder for their research had a dew point of 4°C. After atomization of the melt, the droplets solidify into powder particles and are carried up and out of the spray chamber by the flowing gas.
The powders are transferred to cyclones for particle size classification, followed by powder packaging and shipping to the P/M part producers. A similar atomization system shown is used by Alcan-Toyo America (ATA) in
Napierville, Illinois, for CIGA of aluminum powders (Figure 2.lb) but the spray chamber is isolated from the ambient air. Before atomizing, the spray chamber of a CIGA process is purged with an inert gas to remove residual gases, such as air and water vapor .However, Una1 further commented that the purge gas may not completely remove oxygen and gaseous
water from the spray chamber. The implication of incomplete removal of these residual gases would cause the incorporation of the oxygen and water vapor into the oxide film that naturally forms on nascent aluminum metal . The atomization gas used in the CIGA-ATA atomization plant is a by-product of methane ( C b ) combustion in air . Due to proprietary rights on the part of ATA, detailed information about the exact atomization gas is not available. However, one may speculate that the CIGA-ATA atomization gas is similar to flue gas, a dried gas mixture of carbon dioxide (C02)and nitrogen (N2) gases from the combustion of methane in air  as shown by equation 2.1. Other forms of inert atomization gases are CH4(g) + Air + Heat =+> C02(g) + N2(g) + H20(g)
used in industry for aluminum powder production. Industrial inert gas, which is similar to flue gas, is composed of gas mixtures of carbon dioxide (C02) and nitrogen (N2) gases . Nitrogen gas produced from liquid nitrogen is another source . The vertically downward atomization system (Figure 2.2a) is used by Valimet, Inc. for CIGA-VAL aluminum powders. The spray chamber is isolated from ambient air and is purged before atomization with an inert gas for similar reasons previously mentioned for the CIGA-ATA aluminum powder production process. The molten aluminum is prepared in a furnace and transferred to the melt chamber by a ladle. The melt chamber volume is kept full
to maintain a constant head pressure for the melt to pour into the spray chamber at a constant rate. Upon exiting the pour tube, the molten stream is disintegrated into molten droplets by an atomizing gas nozzle system encircling the pour tube. The used atomization gas is recirculated for reuse to minimize gas consumption costs. Valimet produces two types of aluminum powders, standard spherical aluminum (SSA) and low oxygen (Lox) powders. The SSA powder is produced by gas atomizing the molten aluminum with a gas mixture of helium and a maximum of two volume percent
oxygen . The powder surfaces oxidize in-flight due to a spontaneous reaction between the oxygen in the atomization gas and the nascent aluminum. The Lox powder is made by atomizing with argon gas and passivating the powder in a powder collection vessel by controlled addition of a gas mixture of nitrogen gas and two volume percent oxygen . An alternative inert gas atomization method, and the subject of this research, is gas
atomization reaction synthesis (GARS). The design of the GARS atomization system (Figure 2.2b) is a vertically downward design. The details of the process are described in the Experimental Procedures. In brief, the GARS process uses ultra-high purity (UHP) nitrogen
gas for atomization of the molten stream to partially suppress the inherent oxidation kinetics.
In all of the atomization practices described above, the aluminum powders are oxidized in-flight as they pass through the spray chamber. The degree of powder oxidation is proportional to the oxygen content of the atomization gas. Nyborg and Olefjord [lo] have derived an expression (equation 2.2a) for oxide thickness, tox (A), as a function of partial pressure of oxygen, p(02) (Pa), and reaction time, z (seconds), for a given particle diameter, d (pm). The equation was applied to oxide film growth on ferrous powders during gas atomization, as well as aluminum powder produced by gas atomization [I 13. The constant C (equation 2.2b) in equation 2.2a is composed of terms related to physical and chemical properties of the metal, oxygen, and metal oxide, where pox is the oxide density (kg/m3),
X O , is~ the ~ weight fraction of oxygen in the oxide, R is the universal gas constant (J/mol.K), T, is the gas temperature (K), Mo is the molar weight of elemental oxygen, Sh is the Shenvood number (Sh= 2+0.6Re1/2Pr1/3), and D(02) is the diffusivity of 0 2 in the atomization gas (m2/s). Equation 2.2a corroborates intuition that atomization gases with large oxygen contents, e g , air atomization, create thick oxide films on metal powder
= C.p(O2). 7
During gas atomization of molten metal, the final particle shape is dependent upon several competing reactions including the oxidizing potential of the atomization gas and liquid metal properties of surface tension and viscosity. Powder spheroidization is a function of the viscosity (Om)and surface tension (pm)properties of the aluminum melt that are directly dependent on temperature. Nichiporenko and Naida [121 describe an expression (equation 2.3) for the time to spheroidize, tsph (seconds), a molten droplet that is directly dependent on the melt viscosity, pm (Pas), and inversely dependent on the melt surface tension, Om (N/m), where V (m3) is the powder particle volume, R (m3) is the particle radius after transformation to the spherical shape and r (m3) is the particle radius before the transformation. Two assumptions are made by Nichiporenko and Naida, the ratio of R to r is 10 to 1 and the spheroidization occurs in the absence of oxide film formation. (2.3) Ozbilen et al.  have shown that the volumetric oxygen content of nitrogen atomization gas affects the aluminum powder particle shape. Their atomization experiments show that increases of the oxygen content in a nitrogen-based atomization gas causes the
shape of the powders to become more irregular or less spherical. The limiting volumetric oxygen content of the atomization gas was about three percent oxygen for maintaining spherical or near-spherical shaped powder particles. An argument for the formation of irregular aluminum powders is based on the decrease of surface tension of the molten aluminum in the presence of oxygen [ 141. Ozbilen et al.  also present another argument for the formation of irregular shape of the aluminum
10 powder particles. Their first opinion states that molten aluminum droplets in the presence of a high oxidizing potential gas, such as ambient air, will support a large number of nucleation sites for oxide islands to form on each droplet surface. The oxide islands act as pinning sites, restraining the surface tension forces, thus creating powder particles with irregular shapes. Another argument to support the observation of irregularly shaped aluminum powders is the presence of temperature gradients and compressive stresses in the vicinity of the oxide islands. Because the oxidation of aluminum is an exothermic reaction, the temperature in the region of the oxide may increase, delaying solidification in the region of the oxide. The compressive stresses around the oxide islands develop due to different thermal expansion coefficients of aluminum oxide and aluminum metal. Ozbilen et al. [ 131 cite Spaepen et al.  as showing that compressive stresses reduce the melting point of the aluminum, using the Clapeyron-Clausius relation, delaying the droplet solidification. Such an irregular solidification pattern could interfere with the spheroidization driving force of the surface tension properties. Ozbilen et al. concluded that the oxide film on the aluminum powder surfaces would
vary in thickness, with thick films formed while the droplet was in the liquid state and thin films between the islands formed after solidification. Nyborg and Olefjord [ 161 observed similar oxide film thickness variations in their XPS investigation of an aluminum alloy powder produced by helium gas atomization. Gas atomization conditions, such as pouring temperature, metal flow rate, gas pressure, atomization gas composition and nozzle geometry, affect the aluminum powder size distribution. Unal [ 171 discusses these variables of the gas atomization process that appear to be responsible for the resulting powder size distribution. His conclusions summarize his interpretation of the results for the production of AA 2014 aluminum alloy powder. Pouring temperatures greater than 825°C contribute slightly to decreases in the median powder size due to a reduction of the viscosity and the surface tension of the melt with increasing
11 temperature. The mass median diameter increases proportionally with the square root of the
metal flow rate. An increase of the gas pressure shifts the median powder size to lower values, but beyond a certain gas pressure there are diminishing returns with respect to median particle size. Finally, light weight gases, such as helium gas, reduce the median particle size due to higher gas velocities attainable in supersonic flow conditions. A disadvantage to using helium gas is the unit cost, about 34%more than the cost of nitrogen gas in similar compressed gas cylinders. This expense needs to be balanced against the economic value of a finer powder size distribution. Aluminum Powder Characterization Bulk chemistry
The bulk chemistry of P/M powders is a quality control point used by P/M parts
producers to assure chemical consistency between the different batches of powders shipped to them by the aluminum powder producers. In the case of aluminum P/M, the aluminum alloy composition will determine the elevated metal working temperatures for powder consolidation processes, such as hot isostatic pressing (HIP), vacuum hot pressing (VHP), solid state sintering and liquid phase sintering. If the composition changes from the expected composition, the aluminum P/M parts produced using these types of elevated temperature operations may not meet the design specifications and have to be discarded as scrap.
For example, alloy elements in aluminum metal powder, such as iron, magnesium, silicon, and copper, are known to form low temperature eutectics. If the scheduled temperature of a densification process, such as solid state sintering, is above the solidus of the alloy with the impurities, a liquid phase would form and the consolidated parts would deform. The chain of events would require disposing of the defective parts, decreasing the
yield of P/M parts produced, increasing manufacturing costs, which would be passed on to the consumer.
12 Aluminum powder producers also provide a bulk oxygen content of the aluminum powders. The bulk oxygen content values, though, can be misleading, particularly if the particle size distribution or the surface area of the powders is not available. From a geometrical point of view, if all the oxygen is on the powder surface as an oxide film of uniform thickness and the surface area to volume ratio of the particle increases with decreasing particle size, then the bulk oxygen content increases with decreasing powder particle size. Different researchers have determined with surface analysis methods, e.g., Auger electron spectroscopy (AES)[16, 181 and x-ray photoelectron spectroscopy ( X P S ) [18,
191, that the oxygen is on the surface of the powder particles in the form of oxide films. From these aluminum powder surface investigations, the measured bulk oxygen content appears to arise solely from oxides and water molecules combined within the oxide film. A standard oxygen measurement, such as inert gas fusion (IGF), is unable to distinguish between oxygen associated with an oxide or oxygen from water molecules. Both sources of oxygen, oxides and water, originate from the atomization process, i.e., residual oxygen and water vapor in the atomization gas, the spray chamber andor the powder collection bins. Powder surface area measurements
The surface area of metal powder can be measured by gas adsorption, permeametry,
or from particle size distribution data. The gas adsorption procedure is also known as the
Brunauer-Emmet-Teller (BET) method [20,21]. BET determines the surface area of a powder sample by measuring the amount of gas necessary to cover the powder surface with a monolayer of gas . Typical gases included nitrogen for surface areas greater than one
meter squared per gram or krypton for specific surface area less than one meter squared per gram. A strong attribute of the BET method is its ability to include surface area measurements of interior surface-connected pores . BET measurements are suitable for
13 powder particles of any size and shape. Gas permeametry measures the resistance of a flowing gas through a powder bed . The technique is limited to powder sizes ranging from 0.5 to 50 pm and is only an
approximate measurement tool as it does not assess the dead ended surface connected
porosity . Despite some of the limitations of gas permeametry, the method is simple, reproducible to f 1%, quick, and low cost compared to the equipment costs of other methods, such as BET. A particle size distribution analysis of a powder sample can also provide a calculated
surface area measurement, assuming the shapes of the powder particles are spheres, the powder is not agglomerated, and there are no powder satellites attached to the surface of the powders. If the powder generally meets these requirements, the calculated surface area is a reasonable value .However, the calculated surface area value should not be interchanged with BET measurements, because the calculated surface area does not reflect surfaceconnected porosity or other topographic characteristics of the powder particles .
Aluminum uowder surface characterizations
Surface characterization investigations of aluminum powders typically use instrumentation, such as transmission electron microscopy (TEM) [22,23], A E S [ 11,241, and XPS [11,23,25], to analyze the oxide film. Researchers tend to use various combinations of these techniques for their surface oxide evaluations. Each analytical instrument provides a different view of the same oxide film. TEM can provide information about the oxide chemistry, oxide thickness, and oxide structure, i.e., whether or not the oxide film is crystalline or amorphous. The oxide chemistry can be measured by various methods, e.g., energy dispersive spectroscopy (EDS) and/or parallel energy electron energy loss spectroscopy (PEELS). A bright field image of the oxide film permits direct measurements of the oxide thickness from either individual powder
particles or from the oxide boundary between two powder particles . The oxide structure
can be determined with either secondary area diffraction (SAD) patterns or convergent beam diffraction (CBD) patterns. The difficulty with these last two measurements is focusing the electron beam to a small enough cross-section to minimize detection of neighboring crystalline features. In general, TEM sample preparation is laborious, tedious and time consuming. A E S and X P S , on the other hand, offer relatively simpler sample preparation methods
and provide measurements of the oxide film thickness and oxide film chemistry. Both spectroscopic techniques use argon ions for sputtering, or etching away, successive layers of the oxide film and measuring the elemental composition of each layer. The data is presented
as elemental composition depth profiles of the oxide film on aluminum powder particles. An advantage of A E S is the ability to carry out a point analysis on individual powder particles, providing a comparative measure between fine and coarse powders . The XPS analysis, on the other hand, is an average of many powder particles within a definite area on the order
of one square millimeter. Another type of surface analysis of the oxide film on aluminum powder particles is possible with quadrupole mass spectroscopy (QMS). QMS detects and measures the gases that evolve from the surfaces of the aluminum powder particles during a continuous heating of the powder sample under a dynamic ultra-high vacuum (UHV). The gases typically measured are water and hydrogen, the sources of which comes from water physically adsorbed onto the powder particles' surfaces (physiosorbed water) and water chemically bound within the oxide film (chemisorbed water). In some instances, carbonaceous gases, e.g., carbon monoxide and carbon dioxide, are measured also, but carbon-based gases are more difficult to identify with QMS. The origins of the physiosorbed and chemisorbed water are traceable to the atomization process and post-atomization powder handling [24,25]. Direct comparisons of
15 the QMS results show aluminum alloy powders produced by inert gas atomization have less chemisorbed and physiosorbed water than aluminum alloy powder manufactured by air atomization . A similar type of investigation  used aluminum-magnesium base alloys to show that "wet" atomization gases produce more chemisorbed water in the oxide films of aluminum powder particles than "dry" atomization gases. The same research showed no significant difference ofthe physiosorbed water quantity on the aluminum powders produced by either atomization gas. The hydrogen detected during QMS experiments is a product of the physiosorbed water or chemisorbed water reacting with aluminum cations diffusing through the oxide film [28,29]. Possible reactions for the hydrogen product are shown with equations 2.4,2.5, and
2.6. There is uncertainty and speculation as to which reaction or reactions may be dominant during the heating of the powder sample . One method of hydrogen analysis is a vacuum extraction analysis as described by Peterson et al.  and Devr2ve et al. [313. In brief, the aluminum sample is heated
to a temperature of greater than 600°C and less than 800"C, under vacuum conditions of 3.2~10-2Torr to 1x10-6Torr. The hydrogen evolved from the aluminum specimen is collected in a collection volume of known capacity and the pressure increase within the
collection volume is measured. Once the pressure reaches a constant value, the hydrogen from the sample is inferred to be completely removed. The equilibrium pressure value is directly proportional to the mass content of hydrogen that was in the aluminum sample. Depending on the system available, the hydrogen extraction process is the rate limiting step, and the calculated hydrogen content can be determined within twenty minutes to several
hours . Caution though is warranted for determining the hydrogen content of aluminum. The measured hydrogen content of aluminum ingots may be influenced by several variables, such
as sample porosity, surface contamination, oxide thickness, and grain size . As a result, there are no consistent experimental hydrogen content values for aluminum .
Hydrogen analysis of aluminum powders adds one more variable to the list mentioned in reference , that needs consideration, the water content of the oxide film. Under the elevated temperature and vacuum conditions, the physiosorbed and chemisorbed water would be removed from the oxide film, and if some of the water did not react with aluminum to form hydrogen, the unreacted water would be gathered into the collection volume with the hydrogen. The water in the collection volume would contribute to the measured pressure, leading to an artificially high hydrogen content of the aluminum powder. Exdosibilitv of.aluminumpowders
In 1964, the United States Department of the Interior, Bureau of Mines, prepared a document for the explosibility of metal powders . The report is a standard for all metal powder explosibility testing. The comprehensive investigative report provides explosibility data on 3 13 elemental metal, alloys, catalysts, and ores comprising 54 types of material. An empirical explosibility index (EI) is used to rate each material tested. The E1 value is the mathematical product of the ignition sensitivity (IS) and the explosion severity (ES) (equation 2.7). Table 2.1 lists the relative explosion hazard index with the corresponding index of explosibility ranges. As the information in the table implies, a larger E1 value means a more severe explosion. The ignition sensitivity assumes a dependency on the ignition temperature (IT), minimum ignition energy (MIE), and the minimum explosive concentration (MEC) (equation
2.8). The explosion severity assumes a dependency on the maximum explosion pressure
17 Table 2.1. Legend for the explosive hazard index and the designated range of values for the index of explosibility .
Explosive Hazard Index
Index of Explosibility
None Weak Moderate Strong Severe
(MEP) and maximum rate of pressure rise (MRPR) (equation 2.9). A value of unity is assigned to the explosibility index, ignition sensitivity, and the explosion severity for materials that have similar ignition and explosion characteristics as Pittsburgh seam coal dust. The explosibility tests are conducted in a twenty liter spherical dust explosion chamber as described in reference . The metal powder is dispersed in the air inside the explosion vessel and the explosibility of the metal powder is determined. In the case of MEC values, Safety Consulting Engineers, Inc., advises discretion in the interpretation of the MEC EI = IS* ES
(2.9) values, because the processing conditions and handling of the metal powders strongly
influence the degree of hazard , i.e., the results should be considered "preliminary results" . There are several variables that contribute to dust explosions, such as particle size, particle shape, particle reactivity, distribution in air or gas media, turbulence, size of cloud and confinement, ignition source size, and ignition delay. As an example of one variable effecting dust explosions, aluminum powder particle size has been correlated with MEC
values . The findings show that the MEC becomes more severe with decreasing aluminum powder particle size. The argument for this observation is that small aluminum powder particles have large surface areas compared with the small surface areas of large aluminum powder particles. Hence, for the small aluminum powder particles, there is more area available for a reaction to occur between the aluminum powder particle and the atmospheric air. There is experimental evidence available that indicates nitrogen plays a major role in the combustion of aluminum in air . These authors reference a study by Prentice  that investigated aluminum burning in an argon-oxygen atmosphere during which he observed a clean metal surface, whereas burning in air created an oxide on the powder. Boborykin also reference other research [40,41] conducted in pure nitrogen and oxygen mixtures with argon or nitrogen in which aluminum nitride was formed.
Consolidation of Aluminum Powders Press and hiah interparticle shear consolidation A typical consolidation route that an aerospace PM parts producer would use for
consolidating aluminum alloy powders is shown in Figure 2.3. The sequence begins with the production of gas atomized aluminum powder by one of the commercial methods described at the beginning of this chapter. The as-atomized powder is sieved or pneumatically classified to achieve the desired particle size distribution for cold isostatic pressing (CIP). Ideally, the CIP compact should be pressed to a green density of about 75% of theoretical density to ensure an open porosity network for effective degassing of the aluminum powders . The compaction pressure needed for the ideal green density can be determined from a compressibility curve . After the powder is consolidated by CIP,the green compact is placed in a sealed
aluminum metal can, except for an open vent pipe to allow the escape of water vapor and
Figure 2.3. Conventional consolidation sequence for aluminum powders used in aerospace applications [l]. gaseous hydrogen from the can during the vacuum hot degassing (VHD) procedure. For the sources of hydrogen evolution refer to equations 2.4,2.5, and 2.6 above, and see equation 2.10 and 2.1 1 below for the water vapor sources in the oxide film. The maximum temperature for VHD depends on the solidus temperature of the aluminum alloy powder, which can range from 45OOC to 575OC. The purpose for VHD of the green compact is to eliminate the physiosorbed and chemisorbed water from the oxide film on aluminum powder particles. Equations 2.10 and 2.1 1 describe the dehydration sequence according to the research of Litvintsev and Arbuzova . QMS experimental evidence has shown the oxide film on aluminum powders to be a
duplex structure of alumina (Al2O3) and alumina trihydrate (f!d203.3H20), with physiosorbed water present on the surface of the oxide film . As the green billet is heated to the degassing temperature, the physiosorbed water evaporates from the oxide surface according to equation 2.10. The decomposition reactions of the hydrated alumina phases are represented in equation 2.1 1. The trihydrate phase is thermally stable to about 150°C. Above 150°C and below 175"C, chemisorbed water is removed from the trihydrate phase, forming the A1203.2.5H20 hydrated alumina phase. As the temperature continues to increase from 175°C to 3 1O"C, more chemisorbed water is removed from the d203-2.5H20 phase to form the alumina monohydrate (AI203.H2O) phase. From 3 10°C to 500"C, the monohydrate phase is thermally stable. As the temperature increases above 500"C, the monohydrate phase decomposes to an anhydrous alumina (Al2O3) phase. If the aluminum
20 powder is an aluminum alloy with magnesium additions, the highly mobile and reactive magnesium can react with water to form MgO and hydrogen gas, equation 2.12. (2.10) (2.11)
(2.12) The typical size of the vacuum hot pressing (VHP) cans range from 25 cm to 76 cm in diameter and the billet mass is 50 kg and 1545 kg, respectively [l]. For the small billet sizes, Billman et al. state the VHD is conducted under a dynamic vacuum during heating and a one hour soak at the VHD temperature, the entire process requires about seven hours. For the large billets, the same authors comment that the billets are heated under argon, either static or hot flowing argon, with a one hour vacuum soak near the end of a thirty hour heating cycle. Typical degassing times at degassing temperature vary from twenty-four hours at the periphery of the billet to one hour at the center of the billet. The degassing temperature should be below the solidus of the aluminum alloy powder, and the time at temperature should be limited to minimize coarsening of the microstructure [1,421. Immediately following the VHD procedure, the can is sealed to maintain an
evacuated atmosphere within the interconnected porosity of the green billet [ 11. Billman et al. state that sealing the evacuated sample prevents exposure to air that could react with the
heated P/M billet to form nitrides and oxides within the interconnected porosity. After welding the can closed, the sample is VHP to close the interconnected porosity . Kim continues to comment that the material flow during VHP is adequate to disrupt the dehydrated oxide film into alumina fragments. However, the alumina fragments remain along the prior particle boundaries of the powder particles, leading to incomplete powder particle bonding. Hot extrusion of the VHP billet is necessary to distribute the alumina fragments throughout the matrix. The deformation is completed at extrusion ratios about
20: 1 . The shape of these extrusions can be round bar or rectangular bar. The last step of
the aluminum powder consolidation is the shaping of the final P/M part by closed die forging and/or machining methods. High economic costs are association with the energy consumption necessary to heat the powder samples for VHD, VHP, and hot extruding. The escalated expenditures limit the use of this consolidation procedure to high-tech applications, prohibiting its use for low cost applications, such as automotive drive train components. Press and sinter consolidation
Another method used for consolidating metal powders is a pressing and sintering process (Figure 2.4). After the powder is gas atomized and size classified, the aluminum
Aluminum and Size C1assify
Figure 2.4. Press and liquid phase sintering (LPS) route for aluminum P/M components. powder can follow one of two routes. Either pure aluminum or aluminum alloy powder is immediately die pressed into the component shape or the aluminum powder is blended with elemental or master alloy powders and then die pressed. The blending procedure may involve mixing non-metallic particles, e.g., alumina and silicon carbide, and/or other metal powders, e.g., copper, magnesium, iron, silicon, zinc, for alloy additions. After die pressing, the green component is transferred to a sintering furnace to thermally enhance densification by liquid phase sintering. Solid state sintering is not practiced because of poor fracture resistance related to oxide powder surfaces. The sintered PA4 aluminum part may require
22 secondary finishing operations, such as drilling, milling, turning, and grinding, which are easily performed on aluminum P/M components .
The powders or powder blends that fill the die need to flow well for automated, high production rate presses. The powder particle shape and size affect the flow of the powder into the die. Spherical powders greater than 45 pm in diameter are ideal for die filling, because the powders roll into the die cavity and have low interparticle friction characteristics . Irregular powder particle shapes or fine sphericalpowders have high surface area to
volume ratios that increase the interparticlefriction, decreasing the powder flowability . After filling the die cavity, the aluminum powders are squeezed together to make a densified green compact. The ability of the aluminum powders to deform depends on the compressibility characteristics of the powder or powder blend. The oxide film on aluminum powders is one variable that influences compaction of aluminum P/M parts due to the hardness of the oxide . During the compaction process, the powders deform to fill the empty spaces between the powder particles. The presence of the oxide film can slow the deformation of the particles and even inhibit interparticle bonding. Particle shape and size influence the compressibility of the powders, too. Ideally, a P/M parts producer would use spherical powders with a good mixture of particle sizes for filling the maximum space within the die cavity . However, irregular shaped aluminum powder particles are often
preferred, in spite of reduced die filling capability, because of mechanical interlocking between the powder particles that enhances the green strength of the compact. The inherent hardness of the metal powder is another variable effecting compressibility and is dependent on whether aluminum alloy ("prealloyed") powders or elemental powder alloy blends are used. The elemental powder blends are powder mixtures of aluminum powder with other metal powders, such as copper, magnesium, iron, silicon,
23 and/or zinc. The elemental blends would deform easier at lower compacting pressures than the prealloyed powders  due to the elemental powders being softer and more ductile than the prealloyed aluminum powders. In other words, the prealloyed aluminum powders will
work harden more and faster than the elemental blends, due to the alloy additions in the matrix, requiring higher compaction pressures for the prealloyed powders. Higher green densities and higher green strengths are advantages to using elemental blends for powder compaction  compared to prealloyed powder compacts. The powder compact ejected from the die has green properties that are dependent on the powder and die pressing conditions. The green density of the P/M aluminum component is directly proportional to the compaction pressure applied to the powder. The compacting pressure, compaction method, and the geometry of the P/M aluminum part influence the magnitude of density gradients within the powder compact . The green strength is directly dependent on the green density and the compaction pressure , in other words, as the number of metallurgical bonds created during the die pressing operation increases, the green strength increases. A thick oxide film would inhibit the formation of metallurgical
bonds and lead to poor green properties. Sintering
The green aluminum P/M compact is further densified by sintering, an elevated temperature process to increase the strength of the green compact by bonding adjacent particles by diffusion mechanisms [2 13. P/M aluminum sintering may either occur in the solid state or partial liquid state . The former is rarely used whereas the latter is widely used for either elemental powder blends or blends of aluminum powder with master alloy powders. During solid state sintering, five diffusion mechanisms are possible as shown in Table 2.2. Two of the five mechanisms enhance densification and the other three merely coarsen
24 the microstructure. A major barrier to the solid state sintering process, and diffusion, is the
oxide film thickness on aluminum powder particles , reported to range from 40A to over 200A . The oxide film may break during the pressing operation, creating cold welds between the powder particles. Gutin et al.  make two conclusions from their research. During sintering of lightly oxidized aluminum powders, atoms diffuse over the entire area of contact between the powder particles. On the other hand, during the sintering of severely oxidized aluminum powders, the aluminum atoms diffuse only in the oxide-free zones of the powder particle contacts and the area of interparticle contact does not increase in size. Munir has developed a predictive model that describes the influence of the surface oxide layer on interparticle neck growth, as determined by the relative sintering
Table 2.2. Possible diffusion mechanisms occurring during solid state sintering [2I].
Diffusion Mechanism Volume Surface Vapor Mass Volume Grain Boundary
Source Surface Surface Surface Grain Boundary Grain Boundary
Sink Neck Neck Neck Neck Neck
Comments Coarsening Coarsening Coarsening Densification Densification
and diffusional fluxes, xs and Xd, respectively. The ratio of these fluxes defines the neck growth rate ratio. A neck growth rate ratio greater than one would indicate a retardation of sintering by the oxide layer. If the same ratio is less than or equal to one, sintering continues uninhibited. Table 2.3 is an excerpt from Table 1 in Munir's paper that shows the neck growth rate ratio as function of sintering temperature and the ratio of the oxide thickness (E,) to the particle radius (r). For a given aluminum powder size and sintering temperature, as the oxide film thickness increases, the neck growth is increasingly more difficult. Iron, on the other
hand, would show good sintering behavior, because the neck growth rate ratio is constant or decreases with an increasing &r ratio (Table 2.3). For both these metals, Munir's model correlates well with experimental results of solid state aluminum powder sintering  and
explains the wide spread industrial use of iron-based powder alloys in automotive applications. The successful solid state sintering of metal powders depends on sintering temperature, sintering time, and sintering atmosphere . A limitation to solid state sintering of aluminum powders is the continuous native aluminum oxide on all aluminum powder particles that inhibits diffusion of aluminum atoms between adjacent powder particles. Another limit to sintering temperature is the effect of alloy elements previously
discussed. Table 2.3. Neck growth rate ratio for solid state sintering aluminum and iron powders as a function of temperature and the ratio of the oxide thickness to particle radius . Metal Aluminum Iron
Temperature ("C) 224 660 633 1539
10-5 1 . 7 103 ~ 1 3.3~1012 1.o 1.o
10-3 1 . 7 1033 ~ 3 . 3 1014 ~ 1.o 1.o
10-1 1 . 51~035 3 . 0 1016 ~ 1.o 1.o
Liquid phase sintering (LPS) of aluminum alloy elemental blends enhances densification of the microstructure. The LPS temperature is based on the composition of the
aluminum alloy, typically in the range of 595°C to 625°C [a]. The sintering time ranges from ten to thirty minutes in a variety of sintering atmospheres, dissociated ammonia,
hydrogen, argon,nitrogen, and vacuum .A nitrogen sintering atmosphere is preferred over the other atmospheres, because of the relatively high, as-sintered, mechanical properties of the P/M aluminum parts . Nitrogen gas is also quite economical in large quantities
compared to the other gases available for sintering atmospheres. Another sintering variable related to the sintering atmosphere is the dew point of the protective atmosphere. The recommended dew point is less than -40°C, which corresponds to a maximum moisture content of 120 parts per million by atomic percent . A dew point lower than the recommended value minimizes oxidation during the sintering operation .
26 To reduce the costs of sintering green P/M aluminum parts, researchers have experimented with air sintering. Storchheim  published a paper in which he describes the viability of using convention P/M process equipment to sinter green aluminum P/M parts in air. The initial sintering experiments were generally poor, requiring thorough evaluation of problems related to the powder size distribution, alloy composition, heating rates, sintering times, and lubrication issues. After implementing solutions to address these problems, the air sintered P/M parts had reasonable mechanical properties after using a T-4 heat treat condition.
A goal of aluminum P/M liquid phase sintering is to homogenize a green microstructure composed of an elemental powder blend. Homogenization occurs by the formation of a liquid phase between the elemental constituents, Le., the creation of a short circuit diffusion path between the chemical elements . There is a large chemical potential, and hence a large driving force for chemical homogenization, between the solute powders and the aluminum powders. The presence of the liquid phase also permits rearrangement of the aluminum powder to enhance further densification . The liquid phase sintering process is limited to a small number of aluminum alloy powder blends, such as 601AB and 201AE3 alloy powders. The 601AB alloy is comparable with the composition of the 6061 wrought aluminum alloy and the 201AB alloy has a composition similar to a 2014 wrought aluminum alloy. An advantage of elemental aluminum powder blends is the starting powders can be of high purity, whereas the primary constituents used to make the prealloyed powders may have undesirable impurities. There are disadvantages to liquid phase sintering aluminum alloy elemental powder blends. One drawback is the large scale heterogeneous microstructure that is present in the as-compacted state, which can be exaggerated with blending elemental powders of significantly different sizes. Another downfall to liquid phase sintering is the oxide film on
the aluminum powders may or may not break open during compaction to allow
27 homogenization of the aluminum alloy . In the case where the aluminurn oxide is not disrupted, the oxide film may be too thick for chemical diffusion of aluminum or the elemental constituents through the oxide film. The dimensional control of the P/M compact is a variable that is difficult to maintain during liquid phase sintering. The liquid phase fraction must be small enough to be held by capillary force within the skeleton of the remaining solid phase to retain the compact shape . Coarsening of the microstructure is another problem with liquid phase sintering. The average grain size increases with either the one-half or one-third power of time and is quite sensitive to temperature changes, i.e., elevated temperatures increase grain growth .
Aluminum Alloys, Reinforcement Phases, and Mechanical Properties During the last two decades, P/M processed, high strength aluminum based materials have been designed for elevated temperature use in aerospace applications, such as struts and other structural members. P/M aluminum materials have gained acceptance in critical applications because of their reduced weight and relatively high strength at elevated temperatures. There are two distinct examples of aluminum reinforced P/M materials. One is a uniform blend of aluminum powder and an "extrinsic" dispersoids like silicon carbide or alumina particulates. The other is a rapidly solidified aluminum powder with "intrinsic" dispersoids containing metastable phases such as A6Fe found in AI-Fe-X alloys, where X is another transition metal or rare earth metal. The strength of these two types of reinforced
aluminum powder materials is attributed to the distribution and thermal stability of each phase in the consolidated microstructure. Extrinsic diwersoids: Composites
Extrinsic dispersoids include oxides, carbides, and nitrides that are blended with either pure aluminum or aluminum alloy powders and are bonded during composite
consolidation. An example is Al-SiC(p) alloys processed by blending aluminum alloy powder with SiC(p), typically ranging from 4-10 pm . Composite strength with extrinsic dispersoids is improved over conventional P/M aluminum alloys, but the ductility decreases at elevated temperatures, due to pore opening at the aluminum-dispersoid interface . The ambient temperature ductility of Al-SiC(p) composites is good, but extensive mechanical work is often necessary to provide an adequate level of ductility. The mechanical deformation process decreases the matrix porosity, creates new surface for aluminum powder bonding, and disperses the reinforcement particulates more uniformly. These composites have demonstrated ultimate tensile strengths to about 350 MPa at 200"C, decreasing to about 300 MPa at 260°C .This would indicate that a typical Al-SiC(p) composite could be
used for long durations at 200°C and for short durations at 260°C. Intrinsic dispersoids: Rapidly solidified alloys
Intrinsic dispersoids are hard intermetallic compounds that form within the aluminum matrix during P/M aluminum powder processing, and exist as either equilibrium or metastable compounds. For example, the Al-Fe-X alloys, where X is either vanadium, cerium, cobalt, or molybdenum, have been processed to produce equilibrium A13Fe, its precursors 0'and o",or metastable A16Fe. The ternary additions have high liquid solubility and low solid solubility to promote copious precipitation of the desired intermetallic phases. These aluminum alloys are produced by either gas atomization or melt spinning to promote supersaturation of the alloying elements in the aluminum powder matrix by a rapid solidification process. By controlling the rapid solidification process and fabrication techniques, high volume fractions of finely dispersed intermetallic phases can be produced, giving a dispersion strengthened alloy with high strength and dispersoid thermal stability at elevated temperatures . The size of the dispersoids in a A1-12Fe-2V alloy, Le., o",O',or Al3Fe can vary from 40 to 100 nm . The ultimate tensile strength begins to decrease
29 rapidly from 500 MPa at temperatures greater than 240°C . Cerium additions to the Al-
Fe system have been observed to retard coarsening of the intermetallic phases and suppress the formation of Al3Fe in favor of more stable, high temperature ternary phases , AlloFezCe and AlaFe4Ce . The tensile strength of Al-Fe-Ce alloys begins to decrease significantly from 300 MPa at 290°C [SS] due to microstructural phase coarsening . AlFe-Ce alloys have fair ductility, about 6% elongation at 230"C, and fair toughness at elevated temp.eratures, but thermoniechanical processing improves these properties . All aluminum P/M materials form an oxide surface film on the particles during atomization , requiring extensive mechanical deformation to disrupt the oxide layer and develop adequate interparticle bonding for sufficient ductility. Residual gas contamination within the Ph4 aluminum alloy matrix, such as hydrogen gas, may have deleterious effects on the microstructure and mechanical properties of the aluminum or aluminum alloy P/M component. Kim  discusses how the presence of hydrogen is one variable that influences the microstructure and tensile properties of Al8.4Fe-7.2 Ce, an aluminum alloy produced by gas atomization with flue gas. The tensile properties measured as a function of temperature showed a decrease of tensile strength with increasing temperature. Kim attributes the tensile strength decrease to hydrogen gas released from the decomposition of hydrated oxide fragments. In tension, the neck area relaxes and the newly formed hydrogen assists in crack formation. The size and number of cracks increase with temperature and have the effect of decreasing the cross-sectional area of the tensile specimen.
A New "Hope": Gas Atomization Reaction Synthesis The problems described so far with aluminum powder processing can be minimized
or even eliminated with an atomization method developed at the Ames Laboratory, Gas
Atomization Reaction Synthesis (GARS) . The GARS project had the original intent of
producing intrinsic-like dispersoids in the aluminum matrix by a reaction between the atomization gas and the molten aluminum. The key to manufacturing materials with intrinsic dispersoids is to take advantage of a rapid solidification process, such as gas atomization, which extends the solid solubility in many metal alloy systems. However, instead of an enhanced solute addition to the melt in the crucible, the GARS method adds an excess of a reactive gas solute into the molten aluminum droplet, which is trapped in the rapidly solidified aluminum particle. A dispersion hardened aluminum material can be produced by annealing the supersaturated aluminum powders to promote uniform precipitation of refractory compounds, such as nitrides or carbides, within the aluminum matrix. Ideally, each annealed aluminum powder particle would essentially be a metal matrix composite with refractory dispersoids, similar in nature to Sic, dispersed homogeneously as a highly refined reinforcement particulate. After consolidation of these powders, the result would be an aluminum P/M composite formed by an intrinsic dispersoid precipitation mechanism. To test the GARS process, high-purity aluminum metal was gas atomized with UHP nitrogen gas. The specific goal was to react the nitrogen gas with the aluminum droplets to create a P/M AI-AlN metal matrix composite. During the atomization process, no measurable temperature increases were recorded with a two color optical pyrometer that would indicate an exothermic reaction between the nitrogen gas and the molten aluminum.
Extensive post-atomization analysis of the GARS aluminum powders revealed no conclusive evidence of nitrogen supersaturation of the aluminum matrix or formation of AlN. The reaction between the nitrogen gas and the aluminum metal was apparently by-passed because
of two physical barriers, a) the limited liquid solubility and negligible solid solubility of nitrogen gas in aluminum ,and b) the competition between nitridation and oxidation. Even though gas atomization has the potential to extend the solubility limits of metal alloy systems, any extension of the nitrogen solubility limit in the aluminum-nitrogen system was negligible. The dominant physical barrier to nitridation was oxidation , both from a
thermodynamic argument, i.e., the nitrogen and oxygen Ellingham diagrams [64,65], and
from kinetic evidence .
A re-evaluation of the results from another perspective did reveal the GARS pure aluminum powders to exhibit superior powder characteristics as compared with the CAA, CIGA-ATA, and CIGA-VAL pure aluminum powders. Consequently, the emphasis of the
GARS project shifted to a comprehensive investigation of the "clean" aluminum powder in an effort to exploit its potential for new aluminum P/M processing methods. For example, the GARS aluminum powder has a thinner surface oxide film that may enhance the development of metallurgical bonds during aluminum powder consolidation, especially for solid state sintering operations. The contribution of this dissertation to the aluminum P/M industry is to show the strong linkage between gas atomization processing conditions, asatomized powder characteristics, consolidation behavior, and structure-property relationships
of consolidated pure aluminum powders.
CHAPTER 3. EXPERIMENTAL PROCEDURES To achieve the research goals, four avenues were followed: gas atomization of pure aluminum to produce aluminum metal powder; characterization of the as-atomized aluminum powder; consolidation of the pure aluminum powder; mechanical testing of samples taken from the consolidated specimens. Commercial sources of pure aluminum powder (CAA, CIGA-ATA, and CIGA-VAL) were selected for direct comparative analyses. Two forms of nomenclature will be used throughout the remainder of this dissertation. First, all mass percentages are reported in weight percent. Second, powder size classifications will be denoted with + andor - symbols, the former meaning greater than and the latter meaning less than. An example would be -106+75 pm, which would translate to a powder size distribution of powders nominally less than 106 prn but greater then 75 pm.
Gas Atomization Experiments Atomizer confipuration
Aluminum and aluminum alloy powders were produced in a laboratory scale gas atomizer at the Ames Laboratory. The gas atomization system, shown in Figure 3.1, consisted of three components, the melt chamber, the spray chamber, and the collection system. The melt chamber housed an induction heating system using a graphite susceptor around the exterior of a bottom pouring crucible. The aluminum metal charge was placed in the crucible and the metal was heated through the melting temperature to the selected pouring temperature. The first GARS atomization, GARS-2, used a coarse grained, porous, soft-fired alumina crucible. Due to contamination of the melt from the crucible , the subsequent GARS atomization runs used a fine grained, dense, hard-fired alumina crucible. The change to the latter type of crucible eliminated the problem of tramp element contamination of the metal.
-% &Y Collection
Figure 3.1. Schematic of the gas atomization system used at the Ames Laboratory. After heating the aluminum charge to the pouring temperature, the stopper rod that plugged the hole in the bottom of the crucible was lifted upwards. The molten aluminum poured down through the bottom of the crucible, passed through the pour tube and exited into the spray chamber. The liquid metal stream entering the spray chamber was immediately disintegrated into molten droplets by high pressure gas flowing through a high pressure gas atomization (HPGA-I) nozzle . The HPGA-I nozzle configuration has a ring of twenty discrete jets focused on the molten metal stream such that close-coupled atomization is achieved. As the molten droplets solidify, they fell down the length of the spray chamber and were carried into the collection box by the gas flow. After atomization, the aluminum powder was removed from the collection box and size classified for characterization.
34 Atomization Daranieters
The atomization chamber was evacuated with a roughing pump to a nominal pressure of 50 pnHg to minimize oxygen and water vapor partial pressures. For the GARS-2 to GARS-6 atomization runs (Table 3.la) the atomization system was backfilled to atmospheric pressure with high-purity argon gas before heating the metal charge. For the GARS-7 to GARS-9 atomization runs (Table 3.lb) the atomization system was not backfilled until the metal charge was heated to 500°C. At that point in the heating cycle, the entire system was backfilled to atmospheric pressure with UHP (99.998%) nitrogen gas. This gas had a dew point of less than -67°C. The purpose of the vacuum bake-out was to thermally degas the melt chamber, with the intent of further reducing the level of any gaseous impurities, such as oxygen and water, that may have been present in the atmosphere prior to gas atomization. Table 3.1. Composition, charge mass and pouring temperature of aluminum melts. a. Heated and melted under UHP argon gas. GARS-2 GARS-3 GARS-4 GARS-5 GARS-6 Al A1 A1 Composition A1 AI ChargeMass.(8) 250 900 1510 1400 1600 Pouring Temperature 1400°C 1400°C 950°C 1600°C 1200°C b. Heated under vacuum to 500°C and melted under UHP nitrogen gas. GARS-7 GARS-8 GARS-9 AI-Ti-Y AI A1 A1 A1-3Ti-8.2Y Composition ChargeMass (8) 1533 1760 2100 2200 950°C 1200°C 1400°C Pouring Temperature 1400°C The aluminum melts were atomized with UHP nitrogen gas at a pressure of 6.9 MPa. The pouring temperatures, listed in Tables 3.la and 3.lb, ranged from 950 to 1600°C. Two compositions (Tables 3. l a and 3.1b) were gas atomized for this research, pure aluminum and
an aluminum rich ternary alloy with titanium and yttrium additions. The latter alloy was produced in an attempt to enhance the potential of a nitridation reaction between nitrogen atomization gas and the powder particle. For the GARS-2 and GARS-3 atomization experiments, a high-purity (99.99%)
35 aluminum ingot from NASA was used as the melt stock. For the remaining GARS atomization experiment, the pure aluminum powder was made from a high-purity aluminum ingot (99.999%) from Alcoa. The melt charge mass for each atomization experiment ranged from 250 grams to 2200 grams (Table 3.la and 3.1b). The AI-Ti-Y alloy, listed in Table 3.lb, was made by melting the Alcoa, high-purity aluminum with master alloy buttons of A1-37.2%Ti and A1-91%Y in the melt chamber of the atomizer. The master alloy buttons were made with the Alcoa, high-purity aluminum, 99.80% yttrium from the Ames Laboratory, and 99.99% titanium from Timet. The metal elements were arc melted together to form buttons of the master alloys. The fabrication of the buttons was completed through the Materials Preparation Center at the Ames Laboratory. The purpose for the AI-Ti-Y alloy was an attempt to enhance nitride formation during the gas atomization process between the nitrogen gas and the aluminum alloy. The expectation was additional strong nitride forming elements in the melt would create a nitride phase, resulting with an in-situ metal matrix composite with a stable reinforcement phase. Metallographic Sample Preparation Standard metallographic techniques were used to directly observe the microstructures
of the as-atomized powder particles and consolidated powder samples. The samples were mounted in epoxy using a vacuum infiltration technique. The samples were first ground by hand on grinding paper, Le., 240 grit, 320 grit, 400 grit, and 600 grit, respectively. After each paper, the sample was rinsed with water and rotated 90" before grinding on the next paper. After the 600 grit paper, the polishing continued with the 6 pn diamond spray on a rotating wheel until all the scratches from the 600 grit paper were removed. The samples were then placed on an automated polisher using 6 pn and 1 pn diamond paste polishing compounds, respectively. The diamond pastes helped to remove embedded grinding constituents of previous steps from the soft, aluminum matrix. The final polishing step used
36 a colloidal silica polishing suspension on a Buehler Vibromet 2 with a 10% amplitude
setting. The samples remained on the Vibromet for about 3-6 hours until a majority of the scratches had been removed from the previous polishing step.
Powder Characterizationof Powders Screened at -45 ym Diameter Powder shape and size distribution
The shape of the as-atomized powder particles (GARS, CIGA, and CAA) was assessed with the aid of scanning electronmicroscopy (SEM). To view the loose powders with the SEM, the powders were sprinkled onto conductive carbon tape. Representative micrographs were taken of the loose powders.
A Microtrac I1 size analyzer provided the size distribution of -45pdiameter powders. The apparatus uses laser light scattering to measure the size of particles suspended
in a fluid medium. For the aluminum powders analyzed, the fluid medium was a mixture of one volume percent polyethylene glycol in deionized water. The polyethylene glycol, a surfactant, helped to dispersion agglomerated powder particles into discrete powder particles for more accurate powder size measurements.
The as-atomized aluminum powder densities were measured with pycnometry , a gas adsorption method used to measure the true density of a powder sample. Pycnometry accounts for any internal porosity that may be present inside the powder particles as a result of the gas atomization process. For this research, a Quantachrome MVP-1 Multipycnometer was used and operated according to the manufacturer's instructions listed in the operations manual. The adsorbate gas was ultra-high purity, zero grade (99.999%), helium gas with a .dew point of less than -68°C.
37 Differential thennal analvsis (DTA1
Differential thermal analysis of the as-atomized powders had three intentions: to observe indirectly if the oxide surface film had been destroyed or remained in tact after heating above the melting point of aluminum; to measure the phase transformation
temperatures in the AI-Ti-Y alloy and an Al-4.4%Cu-lS%Mg alloy; to detect any melting point depression in the pure aluminum powders due to impurity elements. The analyses were done with a Perkin-Elmer DTA 7. Before measurements were recorded, the system was purged with argon. The samples were contained in alumina sample holders with heating and cooling rates of 10°C per minute. The pure aluminum, the Al-Cu-Mg alloy and the AI-Ti-Y alloy samples were heated to 700°C, 700°C, and 1200°C, respectively. The analyzed samples were saved for post-analysis examination. The Al-Cu-Mg alloy powder was manufactured by Valimet using a CIGA process with helium plus a maximum of two volume percent oxygen. The Al-Cu-Mg alloy powder was included in this research to observe the effect of magnesium on the vacuum hot degassing process in an aluminum alloy powder, as compared with pure aluminum powder. A DTA scan and quadrupole mass spectroscopic analyses were conducted and compared to draw some conclusions. Bulk powder chemistry
The bulk chemical content was measured with inductively coupled plasma (ICP) using an Applied Research Laboratories ARL 3410 ICP. The metallic elements sought in the pure aluminum samples were silicon, iron, copper, magnesium. These metals are commonly the highest percentage metallic impurities in bulk aluminum. Any abnormally high contents could then be detected with a DTA scan as a freezing point depression. The analysis of the AI-Ti-Y alloy included the same list of elements as above, as well as yttrium and titanium. The oxygen and nitrogen contents of similar powders were measured with inert gas fusion
38 (IGF) using a LECO TC-436 oxygen and nitrogen analyzer. The carbon content was measured by a combustion technique using a Horiba EMIA-520 carbon and sulfur analyzer. The hydrogen contents of the powders were measured by a vacuum extraction technique [313, using instrumentation designed and built at the Ames Laboratory .
Auner electron svectroscopv (AES)
A Perkin-Elmer PHI 660 scanning Auger microscope was used to measure the oxygen concentration profile inwards from the powder surface of the as-atomized powders. Argon ions were used to sputter the surfaces of the powders during depth profiling. For the pure aluminum powders, other depth profiles were made at the same time for the aluminum, nitrogen, and carbon concentrations. For the alloy powders, the respective major alloy additions were added to the profiles, copper and magnesium in the A1-4.4Cu-1 SMg alloy and titanium and yttrium in the AI-Ti-Y alloy. For the analysis of GARS-2 powder, the powder was pressed into indium foil to hold the powder in place. During the analysis, the indium was sputtered and redeposited onto the powder particles, creating inaccurate depth profiles. To eliminate the need for indium foil, a decision was made to make a powder sample that in effect was its own substrate. The powder was cold isostatically pressed (CIP) into a rod shape, nominally 5 cm long, using
6.35 mm diameter rubber bags and pressures of 103.5 MPa to 138 MPa. The first attempts failed to make straight rods. In these cases, the powder would CIP into several small pellets. Success was achieved by placing the bagged powder samples securely into stainless steel sheaths slightly larger in diameter than a CIP bag diameter and maintaining the samples in an upright position during CIP. The bags were secured in the sheaths by folding the ends of the bag over the edge of the sheath and firmly wrapping electrical tape over the bag end and around the sheath. A majority of the samples prepared this way were single straight rods. A section of a CIP rod greater than 16 mm was placed into the Auger and fractured
39 under vacuum to provide a “fresh” surface. Typical analyses consisted of six powder particles, two in the diameter range of 5 to 10 pm, two in the diameter range of 20 to 25 pm diameter, and two in the diameter range of 45 to 50 pn. Powder samples prepared in this fashion eliminated the need to handle loose powders and reduced redeposition problems. Quadrupole mass svectroscouv (0 MS
The QMS system used a lOOC Precision Mass Analyzer, manufactured by Uthe Technology International, to characterize the pure aluminum powders in this study. The gas species of interest were water and hydrogen. The need arose to design and to build a sample chamber capable of minimizing the introduction of atmospheric water and hydrogen into the sample chamber. Figure 3.2 shows the final design and set-up of the sample chamber was connected to the QMS chamber by means of a stainless steel O-ring sealed fitting, Ultra-Torr adapter, made by Cajon. The sample chamber consists of a quartz holding chamber and a quartz furnace crucible connected by the same type of union tee. A type K thermocouple was inserted in the leg of the union tee fitting to approximately measure the temperature of the sample during the analysis. The data generated from these experiments, Le., the sample temperature (“C), the sampling time interval (minutes), system vacuum pressure (Torr) and the intensities of mass currents (amps) of the selected atomic mass units (amu), were collected at 0.25 minute intervals with the aid of a computer. The data acquisition program was written in BASIC by Jim Anderegg, an assistant scientist at the Ames Laboratory. The amu’s selected were 2, 17 and 18 that correspond to hydrogen gas (H2), hydroxide (OH) and water (H20), respectively. The GARS, CIGA-ATA, CIGA-VAL, and CAA aluminum powders were analyzed
by QMS. All aluminum powders samples were densified by CIP at 138 MPa and retained in hermetically sealed CIP bags. The approximate green density of the CIP samples was 8590% of theoretical density, according to the compressibility curve in the ASM handbook
To Roughing Pump
Chamber To QMS
Quartz Holding Chamber Ferritic Stainless Steel Pusher
Figure 3.2. Schematic of the QMS sample chamber used for this research.
. Before each QMS experiment, a piece of a CIP sample was weighed and placed in the holding chamber. The sample weights were between 72 and 185 mg. Small samples were necessary to minimize saturation of the QMS instrumentation. The sample chamber was then evacuated with a roughing pump to 6x10-3 Torr. During this evacuation, the furnace crucible was heated with a hand held heat gun until the thermocouple registered 120°C. This heating assisted in the removal of any adsorbed water
on the crucible walls. After the heated outgassing of the crucible, the furnace crucible cooled to room temperature, and the rough pump valve was closed. The valve between the sample chamber and the QMS chamber was opened, exposing the sample chamber to an ultimate vacuum in the range of 2x10-* Torr. The pumping speed of the turbo-pump was 200 liters per minute. The sample chamber was exposed to this vacuum level for about two hours. During this ambient temperature ultra-high vacuum (UHV) degassing, the sample chamber was monitored with the QMS to measure the relative hydrogen and water levels. After a two hour UHV degassing, the sample was moved, with a ferritic stainless steel pusher, from inside the holding chamber into the furnace crucible, a drop of about 18 cm.
41 The pusher was moved by the motion of a magnet held against the outside wall of the holding chamber without breaking vacuum. Before starting the furnace, the water and hydrogen levels were measured with the QMS for two minutes. The average of these measured intensities were recorded as the initial intensity (Io). After the two minute hold, the furnace was turned on and heated at a specified rate from room temperature to 635°C with an automated, proportioning, Eurotherm 808, controller. Three QMS experiments were done to accurately interpret and validate the results of this analytical technique. One experiment measured the gas evolution due only to the furnace crucible walls and the sheathed thermocouple inside the evacuated crucible, designated as "empty", i.e., no aluminum sample. Another experiment tested a pure hydrated alumina powder sample, A1203.3H20 (99.6%), grade C-33 from Alcoa, to record the relative positions of the water and hydrogen peaks. In this case, the powders were CIP consolidated at 449 MPa in 6.35 mm diameter rubber bags. A small sample, 0.75 mg, was tested to prevent water saturation of the QMS instrumentation. The heating rate for this experiment was 5°C per minute. The third experiment recorded the relative quantities of water and hydrogen evolving from a sample of the Alcoa 99.999% pure aluminum ingot used as the melt stock for the GARS pure aluminum powders. The results of the aluminum powders stimulated two more sets of experiments in an effort to better understand and characterize the QMS analysis technique. One test considered how changes in the heating rate, at constant sample density, would affect the water and hydrogen intensities. The specimen was the CAA aluminum powder CIP consolidated at a density of 92.3% of the pycnometry density, heated at three rates, 2.5"C per minute, 5°C per minute, and 10°C per minute. This powder was selected because of the definitive hydrogen peaks in the QMS spectra. The second examination maintained the heating rate constant, 10°C per minute, and varied the CIP pressure or green density of the CIGA-ATA CIP powders, again, to observe
42 any changes in the relative intensity of the water and hydrogen profiles. This powder was
selected without any established criteria other than its availability and abundance. The densities of these samples, with respect to the pycnometry density, were 71.8%, 83.2%, 86.7%, and 91.7% for CIP pressures of 5 ksi, 15 ksi, 20 ksi, and 30 ksi, respectively. X-rav difiactioii (XRD)of AI-Ti-Y powder
Samples of the AI-Ti-Y alloy powder, at various conditions of heat treatment, were analyzed with a Philips Automatic Powder Diffraction, Model 1729, using copper K a radiation and a scan rate of O.OS"/sec over the range of 15 to 120 degrees two-theta. The phases present in the as-atomized powder were not readily identifiable. To assist with the phase identification, samples of the as-atomized powders were heat treated, one sample at
300°C for 1.25 hours and another at 500°C for 3 hours, to form equilibrium phases within the powder particles. The phases in the heat treated powders were identified using Joint Committee for Powder Diffraction Standards (JCPDS) cards (Table 3.2) and the characteristic peaks were labeled accordingly. The peaks on the XRD trace of the asatomized powder were then identified by overlaying the as-atomized powder scan onto the heat treated XRD trace. Before heat treating, the samples were encapsulated in quartz tubes with a cover gas of argon at a partial pressure of 254 Torr. The encapsulation tubes were then placed in an air furnace for the scheduled time and temperature. After heat treating, the hot samples were removed from the furnace and air cooled. Table 3.2. JCPDS cards used for phase identification in AI-Ti-Y powder alloy. ComDound JCPDS card number A1 04-0787 37- 1449 A13Ti
AIYO~ A15Y30 12
20-0067 29-0103 33-0041
43 Transmission electron svectroscovv (TEM
TEM was used as a complementary tool to AES to validate the oxide thickness measurements as well as determine the structure of the native surface oxide film on pure aluminum powders. Several methods of TEM sample preparation were employed to make foils to show the structure and thickness of the oxide film on aluminum powders. In considering the type of sample needed to accomplish these objectives, a fully dense sample was deemed the best solution. The foil sample needed to have sufficient strength in very thin sections, c100 pn. Also, the consolidation process and sample preparation had to minimize
alteration of the oxide thickness and the native oxide structure, respectively. The powders examined were the GARS-8 and the CAA aluminum powders. The consolidation sequence began with cold isostatically pressing (CIP) the powders at 138 MPa in 2.54 cm diameter rubber CIP bags. The resulting green density was about
90% of the pycnometry density. The samples were then machined to fit inside a cylindrical stainless steel can with a degassing vent pipe welded to the cap of the can, as shown in Figure
3.3. The samples were then degassed in an evacuated electron beam melting (EBM) chamber. The degassing was conducted at room temperature under a vacuum of better than 1x10-6Torr for 24 hours . After degassing and while the sample can was in the EBM chamber, the vent pipe was welded close. The can was then hot isostatic pressed (HIP) at 310 MPa and 300°C for 4 hours. The low HIP temperature was chosen to minimize any oxide phase transformation from an amorphous structure to a crystalline structure which van Beek and Mittemeijer  have observed to occur in the temperature range of 400°C to 450°C. A disadvantage of this sample preparation route is the original oxide film thickness may distort due to the powder deformation. After the HIP cycle, the stainless steel can was removed and 0.8 mm thick disks were cut from the samples. The disks were mechanically ground parallel to a nominal thickness of 0.1 mm on 600 grit grinding paper. Three millimeter diameter foils were mechanically
Powder samples of the GARS-7, GARS-8, and GARS-9 as-atomized aluminum powders were collected for a series of post-atomization oxidation experiments. The powders
were sieved in either a glove bag or glove box under an inert atmosphere and placed in glass vials. The uncapped vials and aluminum powders were then exposed to air with varying amounts of humidity. The exposure times were 0.3 hours, 3 hours, 10 hours, 30 hours, 100 hours, 300 hours, 1000 hours, and 3000 hours. The powder samples exposed for 0.3 hours are designated as the unexposed state. After the designated time of exposure, the sample vials were capped and electrical tape was wrapped around the edge of the cap and vial to ensure no further exposure. The capped vials were stored in a vacuum dessicator box until the bulk oxygen content was measured. The GARS-7 and GARS-8 powders were exposed to air between the months of June and September, in Ames, Iowa, where the indoor humidity ranged from 45% to 50% . The GARS-9 powder collected was evenly divided for two air exposure experiments. One exposure condition was ambient air during the months of December and May with humidity levels between 15% and 25% . The second set of samples was placed in a vacuum dessicator box during the same time period. During this exposure, the dessicator box was filled with a flowing gas of UHP dry air. This experiment was designed to maintain a clean and fresh atmosphere throughout the exposure. The AI-Ti-Y alloy powder was also exposed to ambient air for similar length of times, from the unexposed state to 1000 hours, at nominal temperatures of 25"C, 162"C, and 300°C. The powders exposed at elevated temperatures were placed in quartz tubes closed at one end. The tubes and powders were placed upright in a vertical tube furnace for the specified periods of time. The experiments were conducted indoors between the months of February and May in Ames, Iowa. The relative humidity levels during this time were in the range of
46 Powder explosibility
The MEC of the pure aluminum powders produced for this research were measured with a standard explosibility test chamber as described in references [35,73] at facilities operated by Alcoa in Pittsburgh, PA. The GARS-3, GARS-4, GARS-5, GARS-6 aluminum powders provided preliminary results of the explosibility hazard of samples sieved in air and stored under an inert atmosphere. The time from atomization to the explosibility testing was not accurately measured, nor was the oxide film growth controlled. A more thorough experiment was designed to test the dependence of surface area and oxide film thickness on the explosibility of pure aluminum powders. The as-atomized GARS-9 powder was sieved in a glove box filled with an argon atmosphere into two size ranges, -106+75 pand -38 p.To grow the as-atomized oxide film, the powder samples were exposed to ambient air for 10, 100 and 1000 hours, at either room temperature, nominally 25"C, or 300°C (Table 3.3). The 300°C exposure was completed in a manner Table 3.3. Experimental matrix to evaluate the dependence of oxide film thickness and surface area on the MEC of pure aluminum powders. Sample Powder Size Exposure Time Exposure (w-0 (Hours) Temperature ("C) Indentification -3 8 -38110/25 10 25 -38 -38/10/300 10 300 - 106+75/10/25 -106+75 10 25 - 106+75/10/300 -106+75 10 300 -38 100 25 -3 8/100/25 -38 -38/100/300 100 300 100 25 - 106+75/100/25 -106+75 -106+75/100/300 -106+75 100 300 -3 8 1000 25 -38/1000/25 -38 -38/1000/300 1000 300
-106t75 - 106+75
similar to the thermal oxidation of the AI-Ti-Y powder. At the end of the defined exposure time, several powder characteristics were measured, namely, bulk oxygen content, AES oxide thickness, particle size distribution and MEC. The -38/1000/300 sample was the only 1000 hour exposure sample tested for MEC due to limited financial resources.
Powder Consolidation Consolidationsequence
Due to limited powder quantities, only small consolidated samples could be fabricated. The consolidation of the pure aluminum powders followed a modified consolidation route (Figure 3.4a) [67,74], typically used for aerospace aluminum powder components (Figure 3.4b) [l]. The consolidation experiments used the GARS4 aluminum powders and CAA pure aluminum powder from Alcoa. Rubber CIP bags, 2.54 cm diameter, were filled with -45pm powder to a nominal height of 8 cm. Following the CIP at 138 MPa, the CIP samples were machined to fit into stainless steel cans (Figure 3.3) with dimensions of 1.90 cm diameter, 5 cm tall and a wall thickness of 0.055 cm. Prior to welding the can closed, a vent pipe for the subsequent outgassing treatment was installed on the top of the can. Two degassing procedures, vacuum hot degassing (VHD) and vacuum cold degassing (VCD), were conducted prior to HIP of the aluminum powders. The VHD treatment consisted of heating the sample and HIP can to a temperature of 550°C under a vacuum of 1x10-6to 1x10-7 Torr for four hours. After the VHD, the vacuum furnace was backfilled with UHP argon gas. The sample was removed from the furnace and placed in an argon filled zip-lock bag. The sample was immediately transported to an electron beam melting chamber and evacuated again at room temperature. After evacuating the sample overnight, about 16 hours, to a similar vacuum level as before, the vent pipe was welded shut. The VCD approach involved a room temperature evacuation of the powder sample and can in the electron beam melter over a period of about 16 hours at a vacuum level ranging from 1 ~ 1 0 - ~ to 1x10-7 Torr. The vent pipe was then welded shut. All the sealed evacuated cans were then HIP at 550°C and 310 MPa for four hours. Sections of these consolidated samples were prepared for metallographic examination. The remaining pieces were fabricated into mechanical property test specimens. Specimens of the GARS4 and CAA, each consolidated
a. Modified consolidation sequence for aluminum powders used for this research.
Vacuum Hot Press
b. Conventional consolidation sequence for aluminum powders used in aerospace applications as described in [l]. Figure 3.4. Consolidation sequences of aluminum powder. by either the CIP-VHD-HIP or the CIP-VCD-HIP processing route, were evaluated with QMS. The consolidated sample densities were measured by hydrostatic immersion also referred to as Archimedes method. The density, p (g/cm3), of the sample is determined according to equation 3.1, where Mdry (grams) is the weight of the sample in air and Mwet (grams) is the weight of the sample measured in a fluid of known specific gravity, SGfluid (gkm3). Because some samples were porous, all the surfaces of the samples were lightly sprayed with a polyurethane varnish to prevent water infiltration into the pore network of the consolidated powder product.
49 Post consolidation heat treatment
To test the applicability of the VCD procedure to aluminum P/M components used at elevated temperatures, sections of the GARS-4, CIGA-ATA, and CAA CIP-VCD-HIP samples were heat treated at 300°C for one hour. A similar experiment was conducted on another section of the CAA CIP-VCD-HIP sample heat treated at 550°C for one hour. The CIP-VCD-HIP samples were encapsulated in quartz tubes under an argon partial pressure of 10 inches of Hg. The tubes were placed in a muffle air furnace at the appropriate temperature and held for one hour. Sections of the heat treated samples were prepared for mechanical property testing and for QMS evaluation. Both these examinations made direct comparisons between the non-heat treated and the heat treated samples.
Mechanical Property Measurements Punch testing
The small size of the consolidated samples and the need to maximize the statistical results of the mechanical properties required the use a small punch test. Punch testing  is a method for measuring a select group of mechanical properties from a load versus deflection curve. The raw data was initially recorded on x-y chart recorder paper. Later, a computer collected the data for faster and easier data analysis. The measurable properties from the raw data are coupon thickness, to (mm), yield load, Pyield (N), maximum load, Pmax(N), fracture
energy in Ef(N-mm), and fracture deflection, 6f(mm). With the aid of empirical equations
3.2 and 3.3, yield stress, oyield (MPa), and fracture strain, &f( d m m )were calculated,
respectively. Figure 3.5 is used for the following description to show how the punch test data was determined. The yield load was determined as the intersection of the two tangents shown on the punch test curve. The maximum load was defined at the point were the slope of the curve was zero. For direct relative comparisons, the deflection at maximum load was arbitrarily
chosen as the point of fracture deflection. The fracture energy value required a measurement
of the area under the load-deflection curve, as shaded in Figure 3.5. The CIP-VHD-HIP, CIP-VCD-HIP and CIP-VCD-HIP-heat treated samples were cut transversely into 0.8 mm thick disks and then mechanically ground with 600 grit grinding paper to a nominal 0.6 mm thickness. Each disk yielded three, 6 mm diameter test coupons that were cut using a plunging electrodischarge machining (EDM) technique. The test coupons were ground to a nominal thickness),t(
of 0.500~0.010mm on 1500 grit grinding
paper. The 6 mm diameter coupons were tested with a punch speed of 0.127 cm per minute.
Deflection, 6 (mm) Figure 3.5. Example of the punch test raw data as recorded on a load-deflection curve.
CHAPTER 4. EXPERIMENTAL RESULTS Powder Characterization of -45 pm Diameter As-atomized Powders Shape and size distribution
'The shape of the aluminum powders is idiosyncratic with the gas atomization method used to manufacture the aluminum powders. To illustrate these idiosyncrasies of the CAA, CIGA-ATA and GARS atomization processes, SEM micrographs were taken of the asatomized powder particle shapes. The shape of the GARS aluminum powder is spherical (Figure 4.1) with some satellites, Le., small powders attached to larger particles and agglomerations of small particles. The CIGA-ATA powders (Figure 4.2) range from spherical to irregular shapes. The CAA powders (Figure 4.3) have a ligmental or irregular shape. Table 4.1 shows a list of parameters describing the size distributions of the GARS,
Figure 4.1. SEM photograph of GARS aluminum powder.
Figure 4.2. SEM micrograph of the as-atomized CIGA-ATA pure aluminum powder.
Figure 4.3. SEM micrograph of the as-atomized CAA aluminum powder.
53 CIGA-ATA, and CAA pure aluminum powders. The same table shows the size distribution of the AI-Ti-Y alloy powders manufactured with the GARS technology. The columns are the percentile points, d16, d50, and d84, which indicates the measured volume percent of powder which is smaller than the indicated size. The CSA column is the calculated surface area as determined with the Micro Trac I1 software. Figure 4.4 shows pictorially the size distribution of the GARS-4, CIGA-ATA, CIGA-VAL, and CAA aluminum powders. The GARS-4 aluminum powder, a representative of the other GARS powders, was selected for this figure, because this powder was used in the consolidation and QMS experiments for comparison with the CIGA-ATA and CAA powders. Table 4.1. Particle size distribution data from a Microtrac 11particle size analyzer. d84 CSA Powder d16 d50 Type (PI (PI (PI (m2/cm3> 24.16 12.15 41.87 0.330 GARS-3 23.45 10.66 44.94 0.356 GARS-4 21.40 39.38 GARS-5 10.85 0.364 25.43 46.58 0.325 GARS-6 12.01 27.89 47.37 0.280 GARS-7 14.25 0.328 26.50 46.50 GARS-8 12.28 24.29 0.343 12.23 39.95 GARS-9 20.43 35.14 0.402 AI-Ti-Y 10.20 21.79 41.40 0.35 1 10.1 1 CIGA-VAL 0.33 1 22.16 39.23 CAA 12.08 11.09 1.676 2.17 4.99 CIGA-ATA The size distribution data for the CAA aluminum powder is erroneous due to the
irregular shape of the powder as observed with the SEM micrograph in Figure 4.3. The algorithm used by the computer software of the Micro Trac I1 instrumentation uses the assumption that all powder particles passing through the laser light are spherical. The contribution of each irregular shaped particle to the overall light scattering pattern depends greatly on the orientation of the irregular shaped particle with respect to the laser beam . Kaye and Trottier continue to explain that irregular shaped particles presented to the laser from the broadest side, in effect, distorts the coarse end of the size distribution, making the
size distribution appear more coarse. On the other hand, irregular shaped particles having a parallel orientation to the incident beam has the effect of overestimating the quantity of fines in the size distribution. For irregular shape powder particles, the Micro Trac I1 assigns an
apparent spherical powder size based on the "diameter" of the projected area of the powder particle on the detector of the Micro Trac I1 instrumentation. 100
.. .. .. . ... .. .. ... ..
... ... ... ... ... ... ... ... .... .... .... .... .... .... .... .... .. .. .. .. .. .. .. .. .... .... .... .... .... .... .... ..... .. .. .. .. .. .. .. .. ... ... ... ... ... ... ... ... .. .. .. .. ..
... ... ... ... ... ... ... .......
Particle Diameter (pm)
... ... ...
.. . ... .. .. _ . .... .. ....
. ... .... ..
.... ... .... ... ... ... * .. ... ...
... ... ... ... .:.. ... ...
Figure 4.4. Cumulative size distributions of the GARS-4, CIGA-ATA, CIGA-VAL, and CAA aluminum powders. Densih, measurements and specific surface area
The powder density and specific surface area measurements are two more characterization methods to describe the aluminum powders. The powder density, measured with pycnometry, was determined to assess the theoretical density of the aluminum powders listed in Table 4.2. The standard deviation of the density values for the all the aluminum powders is less than 0.5% of the measured value. The measured density values of the pure aluminum powders are slightly different than the theoretical density of aluminum, 2.70 grams per cubic centimeter. The difference is possibly due to trace element chemical variations within the powders. Another possible reason for the difference are errors in the pycnometry
55 calibration values which are used for the calculation of the pycnometry density.
Table 4.2 also lists the specific surface areas of the powders. The specific surface areas were determined from either BET surface area measurements or calculated from the particle size distribution data and the pycnometry density. The calculated specific surface area, in this case, is the quotient of the CSA column in Table 4.1 divided by the respective pycnometry density value in Table 4.2. Table 4.2. Pycnometry density and specific surface areas of aluminum powders. Powder Pycnometry Density Surface Area Determination (g/cm3) (m%) of Surface Area GARS-3 2.6521-0.007 0.122 Calculated GARS-4 2.641k0.013 0.131 Calculated GARS-5 2.655k0.008 0.134 Calculated GARS-6 2.693k0.005 0.120 Calculated GARS-7 2.6771-0.007 0.103 Calculated GARS-8 2.670k0.005 0.121 Calculated GARS-9 2.7001-0.008 0.127 Calculated AI-Ti-Y 2.8 10+0.009 0.143 Calculated CIGA-VAL 2.6591-0.006 0.132 Calculated CAA 2.699~0.004 0.680 BET CIGA-ATA 2.66720.0 05 0.619 BET Pure aluminum powder analvtical characterization
Bulk chemistq Bulk chemistry measurements provide chemical information about the aluminum powders which is relevant to three areas of aluminum powder processing, i.e., atomization, consolidation, and mechanical property data interpretations. For this research, bulk chemical measurements were made of the GARS melt stock before atomization and the as-atomized GARS aluminum powders after atomization. These measurements help identify problems related to reactions between the molten aluminum and the refractory materials in contact with.
the liquid aluminum. Consolidation procedures should also be properly selected as the chemistry of the aluminum powders would affect elevated temperature processes. For example, elevated levels of trace elements may combine with the aluminum to form low
melting point eutectic phases which could distort a consolidated component, creating a scrap work piece and decreasing the component output yield. Another benefit of a bulk chemical analysis is to assist with a proper interpretation of a chemical dependent mechanical property data, such as yield stress. The melt stock bulk chemistries are summarized in Table 4.3. The NASA aluminum was measured at the Ames Laboratory with Laser Ion Mass Spectroscopy (LIMS) and the Alcoa ingot was measured at Alcoa using Gas Discharge Mass Spectroscopy (GDMS). Both methods of chemical analysis scan the entire period table of the elements and, hence, are semi-quantitative. In other words, the data is a first approximation of the actual chemistry. Note, the GARS-2 and GARS-3 powders were produced from the NASA aluminum ingot
and the remaining GARS powders were manufactured with the Alcoa aluminum ingot. Table 4.3. Bulk chemical measurements of melt stock for GARS aluminum powders. The NASA aluminum was measure by LIMS and the Alcoa was measured by GDMS. N Element A1 cu C 0 Mg Si Fe (ppmw) (ppmw) (ppmw) ( P P ~ W ) (ppmw) (ppmw) (ppmw) (ppmw)